1,540 psi 
Overlap shear strength 



Maple 

23°C 
Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375".The separation rate of the testing jaws was 2" per minute. 
1,890 psi 
Overlap shear strength 



FRP 

23°C 
Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375". The separation rate of the testing jaws was 2" per minute. 
2,100 psi 
Overlap shear strength 



Polycarbonate 

23°C 
Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375". The separation rate of the testing jaws was 2" per minute. 
1,330 psi 
Overlap shear strength 



Polyacrylic 

23°C 
Substrate Failure, Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375". The separation rate of the testing jaws was 2" per minute. 
710 psi 
Overlap shear strength 



Polystyrene 

23°C 
Substrate Failure, Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375". The separation rate of the testing jaws was 2" per minute. 
1,350 psi 
Overlap shear strength 



ABS 

23°C 
Substrate failure, Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375". The separation rate of the testing jaws was 2" per minute. 
1,670 psi 
Overlap shear strength 



PVC 

23°C 
Substrate Failure, Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375". The separation rate of the testing jaws was 2" per minute. 
340 psi 
Overlap shear strength 



Maple 

82°C 
Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375". The separation rate of the testing jaws was 2" per minute. 
800 psi 
Overlap shear strength 



FRP 

82°C 
Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens.These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375". The separation rate of the testing jaws was 2" per minute. 
340 psi 
Overlap shear strength 
10,080 min 
25°C 
50 % 
FRP 
600 sec 
23°C 
FRP, Overlap Shear Strength (psi), tested @ 73°F (23°C) at various times after bonding. The FRP was conditioned for 7 days at 77°F (25°C)/50% RH prior to bonding. 
610 psi 
Overlap shear strength 
10,080 min 
25°C 
50 % 
FRP 
3,600 sec 
23°C 
FRP, Overlap Shear Strength (psi), tested @ 73°F (23°C) at various times after bonding. The FRP was conditioned for 7 days at 77°F (25°C)/50% RH prior to bonding. 
1,910 psi 
Overlap shear strength 
10,080 min 
25°C 
50 % 
FRP 
86,400 sec 
23°C 
FRP, Overlap Shear Strength (psi), tested @ 73°F (23°C) at various times after bonding. The FRP was conditioned for 7 days at 77°F (25°C)/50% RH prior to bonding. 
1,890 psi 
Overlap shear strength 
10,080 min 
25°C 
50 % 
FRP 
604,800 sec 
23°C 
FRP, Overlap Shear Strength (psi), tested @ 73°F (23°C) at various times after bonding. The FRP was conditioned for 7 days at 77°F (25°C)/50% RH prior to bonding. 
1,372 psi 
Overlap shear strength 



Maple 

23°C 
Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375".; The separation rate of the testing jaws was 2" per minute. 
1,199 psi 
Overlap shear strength 



FRP 

23°C 
Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375".; The separation rate of the testing jaws was 2" per minute. 
1,374 psi 
Overlap shear strength 



Polycarbonate 

23°C 
Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375".; The separation rate of the testing jaws was 2" per minute. 
1,219 psi 
Overlap shear strength 



Polyacrylic 

23°C 
Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375".; The separation rate of the testing jaws was 2" per minute.; Substrate failure. 
1,213 psi 
Overlap shear strength 



ABS 

23°C 
Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375".; The separation rate of the testing jaws was 2" per minute.; Substrate failure. 
1,795 psi 
Overlap shear strength 



PVC 

23°C 
Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375".; The separation rate of the testing jaws was 2" per minute. 
499 psi 
Overlap shear strength 



Maple 

82°C 
Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375".; The separation rate of the testing jaws was 2" per minute. 
421 psi 
Overlap shear strength 



FRP 

82°C 
Overlap shear (OLS) strengths were measured on 1" wide 1/2" overlap specimens. These bonds were made individually using 1" x 4" sample coupons. The thickness of the bond line was .003.006". The thickness of the substrates were: plastics, .125", Maple, .375".; The separation rate of the testing jaws was 2" per minute. 
117 psi 
Overlap shear strength 
10,080 min 
25°C 

FRP 
600 sec 
23°C 
FRP, Overlap Shear Strength (psi), tested @ 73°F (23°C) at various times after bonding. The FRP was conditioned for 7 days at 77°F (25°C)/50% RH prior to bonding. 
250 psi 
Overlap shear strength 
10,080 min 
25°C 

FRP 
3,600 sec 
23°C 
FRP, Overlap Shear Strength (psi), tested @ 73°F (23°C) at various times after bonding. The FRP was conditioned for 7 days at 77°F (25°C)/50% RH prior to bonding. 
1,035 psi 
Overlap shear strength 
10,080 min 
25°C 

FRP 
86,400 sec 
23°C 
FRP, Overlap Shear Strength (psi), tested @ 73°F (23°C) at various times after bonding. The FRP was conditioned for 7 days at 77°F (25°C)/50% RH prior to bonding. 
1,199 psi 
Overlap shear strength 
10,080 min 
25°C 

FRP 
604,800 sec 
23°C 
FRP, Overlap Shear Strength (psi), tested @ 73°F (23°C) at various times after bonding. The FRP was conditioned for 7 days at 77°F (25°C)/50% RH prior to bonding. 